A refractory material or refractory is a material that is resistant to decomposition by heat, pressure, or chemical attack, and retains strength and form at high temperatures. Refractories are polycrystalline, polyphase, inorganic, non-metallic, porous, and heterogeneous. They are typically composed of oxides or non oxides like carbides, nitrides etc. of the following materials: silicon, aluminium, magnesium, calcium, and zirconium. Some metals with melting points >1850 °C like niobium, chromium, zirconium, tungsten, rhenium, tantalum etc. are also considered refractories.
ASTM C71 defines refractories as "...non-metallic materials having those chemical and physical properties that make them applicable for structures, or as components of systems, that are exposed to environments above 1,000 °F (811 K; 538 °C)."
Refractory materials are used in furnaces, kilns, incinerators, and reactors. Refractories are also used to make crucibles and moulds for casting glass and metals and for surfacing flame deflector systems for rocket launch structures. Today, the iron- and steel-industry and metal casting sectors use approximately 70% of all refractories produced.
Refractory materials must be chemically and physically stable at high temperatures. Depending on the operating environment, they must be resistant to thermal shock, be chemically inert, and/or have specific ranges of thermal conductivity and of the coefficient of thermal expansion.
The oxides of aluminium (alumina), silicon (silica) and magnesium (magnesia) are the most important materials used in the manufacturing of refractories. Another oxide usually found in refractories is the oxide of calcium (lime). Fire clays are also widely used in the manufacture of refractories.
Refractories must be chosen according to the conditions they face. Some applications require special refractory materials. Zirconia is used when the material must withstand extremely high temperatures. Silicon carbide and carbon (graphite) are two other refractory materials used in some very severe temperature conditions, but they cannot be used in contact with oxygen, as they would oxidize and burn.
Binary compounds such as tungsten carbide or boron nitride can be very refractory. Hafnium carbide is the most refractory binary compound known, with a melting point of 3890 °C. The ternary compound tantalum hafnium carbide has one of the highest melting points of all known compounds (4215 °C).
Refractories have multiple useful applications. In the metallurgy industry, refractories are used for lining furnaces, kilns, reactors, and other vessels which hold and transport hot mediums such as metal and slag. Refractories have other high temperature applications such as fired heaters, hydrogen reformers, ammonia primary and secondary reformers, cracking furnaces, utility boilers, catalytic cracking units, air heaters, and sulfur furnaces.
Refractories are classified in multiple ways, based on:
Acidic refractories are generally impervious to acidic materials but easily attacked by basic materials, and are thus used with acidic slag in acidic environments. They include substances such as silica, alumina, and fire clay brick refractories. Notable reagents that can attack both alumina and silica are hydrofluoric acid, phosphoric acid, and fluorinated gases (e.g. HF, F2). At high temperatures, acidic refractories may also react with limes and basic oxides.
Basic refractories are used in areas where slags and atmosphere are basic. They are stable to alkaline materials but can react to acids. The main raw materials belong to the RO group, of which magnesia (MgO) is a common example. Other examples include dolomite and chrome-magnesia. For the first half of the twentieth century, the steel making process used artificial periclase (roasted magnesite) as a furnace lining material.
These are used in areas where slags and atmosphere are either acidic or basic and are chemically stable to both acids and bases. The main raw materials belong to, but are not confined to, the R2O3 group. Common examples of these materials are alumina (Al2O3), chromia (Cr2O3) and carbon.
These have standard size and shapes. These may be further divided into standard shapes and special shapes. Standard shapes have dimension that are conformed by most refractory manufacturers and are generally applicable to kilns or furnaces of the same types. Standard shapes are usually bricks that have a standard dimension of 9 in × 4.5 in × 2.5 in (229 mm × 114 mm × 64 mm) and this dimension is called a "one brick equivalent". "Brick equivalents" are used in estimating how many refractory bricks it takes to make an installation into an industrial furnace. There are ranges of standard shapes of different sizes manufactured to produce walls, roofs, arches, tubes and circular apertures etc. Special shapes are specifically made for specific locations within furnaces and for particular kilns or furnaces. Special shapes are usually less dense and therefore less hard wearing than standard shapes.
These are without definite form and are only given shape upon application. These types are better known as monolithic refractories. The common examples are plastic masses, Ramming masses, castables, gunning masses, fettling mix, mortars etc.
Dry vibration linings often used in Induction furnace linings are also monolithic, and sold and transported as a dry powder, usually with a magnesia/alumina composition with additions of other chemicals for altering specific properties. They are also finding more applications in blast furnace linings, although this use is still rare.
Refractory materials are classified into three types based on fusion temperature (melting point).
Refractoriness is the property of a refractory's multiphase to reach a specific softening degree at high temperature without load, and is measured with a pyrometric cone equivalent (PCE) test. Refractories are classified as:
Refractories may be classified by thermal conductivity as either conducting, nonconducting, or insulating. Examples of conducting refractories are SiC and ZrC, whereas examples of nonconducting refractories are silica and alumina. Insulating refractories include calcium silicate materials, kaolin, and zirconia.
Insulating refractories are used to reduce the rate of heat loss through furnace walls. These refractories have low thermal conductivity due to a high degree of porosity, with a desired porous structure of small, uniform pores evenly distributed throughout the refractory brick in order to minimize thermal conductivity. Insulating refractories can be further classified into four types:
All refractories require anchorage systems such as wire formed anchors, formed metal (for example, hexmetal) or ceramic tiles to support the refractory linings. The anchorage used for refractories on roofs and vertical walls are more critical as they must remain able to support the weight of refractories even at the elevated temperatures and operating conditions.
The commonly used anchorages have circular or rectangular cross-sections. Circular cross-sections are used for low thickness refractory and they support less weight per unit area; whereas the rectangular cross-section is used for high thickness refractory and can support higher weight of refractory per unit area. The number of anchors depends on operating conditions and the refractory materials. The choice of an anchor's material, shape, quantity, and size has significant impact on the useful life of the refractory.
Tundish boards don't require metallic anchors, rather they are stick together by a special refractory paste and powder. Good practice is to use a combination of paste and powder to make sure the system is leak proof and hold itself together while long duration of castings.
|Wikimedia Commons has media related to Refractory materials.|